View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
1.
Chapter 3
Rolling of metals
Subjects of interest
• Introduction/objectives
• Rolling mills
• Classification of rolling processes
• Hot rolling
• Cold rolling
• Forces and geometry relationships in rolling
• Simplified analysis of rolling load: Rolling variables
• Problems and defects in rolled products
• Rolling-mill control
• Theories of cold rolling
• Theories of hot rolling
• Torque and power
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
2.
Objectives
• This chapter provides information on different types of metal
rolling processes which can also be divided in to hot and cold
rolling process.
• Mathematical approaches are introduced for the
understanding of load calculation in rolling processes.
• Finally identification of defects occurring during and its
solutions are included.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
3.
Introduction- Definition of rolling process
• Definition of Rolling : The process
of plastically deforming metal by
passing it between rolls.
• Rolling is the most widely used
forming process, which provides high
production and close control of final
product.
www.world-aluminium.org
Rolling process
• The metal is subjected to high
compressive stresses as a result of
the friction between the rolls and the
metal surface.
Note: rolling processes can be mainly divided
into 1) hot rolling and 2) cold rolling.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
4.
Introduction- Hot and cold rolling processes
www.vatech.at
Hot rolling
• The initial breakdown of
ingots into blooms and billets
is generally done by hot-rolling.
This is followed by further hotrolling into plate, sheet, rod, bar,
pipe, rail.
Cold rolling
• The cold-rolling of metals has
played a major role in industry by
providing sheet, strip, foil with
good surface finishes and
increased mechanical strength
with close control of product
dimensions.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
5.
Sheet rolling machines
Rolled strips
Rollforming machine
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
6.
Bloom
Billet
Slap
Terminology
• Bloom is the product of first breakdown of ingot
(cross sectional area > 230 cm2).
Semifinished
products
• Billet is the product obtained from a further reduction by hot rolling
(cross sectional area > 40x40 mm2).
• Slab
Further
rolling
steps
is the hot rolled ingot
(cross sectional area > 100 cm2 and with a width ≥ 2 x thickness).
Plate
Sheet
Strip
• Plate is the product with a thickness > 6 mm.
Mill
products
• Sheet is the product with a thickness < 6 mm and width > 600 mm.
• Strip
is the product with a thickness < 6 mm and width < 600 mm.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
7.
Mill rolls
Rolls
Mill rolls
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
8.
Ring rolls
• Ring rolls are used for tube rolling,
ring rolling.
• Ring rolls are made of spheroidized
graphite bainitic and pearlitic matrix or
alloy cast steel base.
Cantilever mill roll
Suranaree University of Technology
Tube mill roll
Tapany Udomphol
Universal roll
Jan-Mar 2007
9.
Typical arrangement of rollers for rolling mills
Two-high mill, pullover
Four-high mill
The stock is
returned to the
entrance for
further reduction.
Two-high mill, reversing
The work can be
passed back and forth
through the rolls by
reversing their
direction of rotation.
Three-high mill
Consist of upper and
lower driven rolls and
a middle roll, which
rotates by friction.
Suranaree University of Technology
Tapany Udomphol
Small-diameter rolls
(less strength &
rigidity) are
supported by
larger-diameter
backup rolls
Cluster mill or
Sendzimir mill
Each of the work
rolls is supported
by two backing
rolls.
Jan-Mar 2007
10.
Typical arrangement of rollers for rolling mills
Continuous rolling
σb
σf
• Use a series of rolling mill and
each set is called a stand.
• The strip will be moving at
different velocities at each
stage in the mill.
A four stand continuous mill or tandem mil.
• The speed of each set of rolls is synchronised so that the input speed of
each stand is equal to the output speed of preceding stand.
• The uncoiler and windup reel not only feed the stock into the rolls and coiling up
the final product but also provide back tension and front tension to the strip.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
11.
Typical arrangement of rollers for rolling mills
Planetary mill
• Consist of a pair of heavy backing rolls
surrounded by a large number of planetary rolls.
• Each planetary roll gives an almost constant
reduction to the slab as it sweeps out a circular
path between the backing rolls and the slab.
• As each pair of planetary rolls ceases to have
contact with the work piece, another pair of rolls
makes contact and repeat that reduction.
• The overall reduction is the summation of a
series of small reductions by each pair of rolls.
Therefore, the planetary mill can hot reduces a
slab directly to strip in one pass through the mill.
• The operation requires feed rolls to introduce the
slab into the mill, and a pair of planishing rolls on
the exit to improve the surface finish.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
12.
Rolling mills
Rolling mill is a machine or a factory for
shaping metal by passing it through rollers
A rolling mill basically consists of
• rolls
• bearings
• a housing for containing these parts
• a drive (motor) for applying power to the rolls and controlling the speed
• Requires very rigid
construction, large motors
to supply enough
power (MN).
Modern rolling mill
• skills
• engineering design
• construction
Suranaree University of Technology
Successive stands of a
large continuous mill
+
Huge capital investment
Tapany Udomphol
Jan-Mar 2007
13.
Different types of rolling processes
There are different types of rolling processes as listed below;
• Continuous rolling
• Transverse rolling
• Shaped rolling or section rolling
• Ring rolling
• Powder rolling
• Continuous casting and hot rolling
• Thread rolling
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
14.
Conventional hot or cold-rolling
The objective is to decrease the thickness of the metal with an
increase in length and with little increase in width.
• The material in the centre of the sheet
is constrained in the z direction (across
the width of the sheet) and the
constraints of undeformed
shoulders of material on each side of
the rolls prevent extension of the sheet
in the width direction.
• This condition is known as plane
strain. The material therefore gets
longer and not wider.
σy
σx
σz
Suranaree University of Technology
• Otherwise we would need the width
of a football pitch to roll down a steel
ingot to make tin plate!
Tapany Udomphol
Jan-Mar 2007
15.
Transverse rolling
• Using circular wedge rolls.
• Heated bar is cropped to length and
fed in transversely between rolls.
• Rolls are revolved in one direction.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
16.
Shaped rolling or section rolling
• A special type of cold rolling in
which flat slap is progressively bent
into complex shapes by passing it
through a series of driven rolls.
• No appreciable change in the
thickness of the metal during this
process.
• Suitable for producing moulded
sections such as irregular shaped
channels and trim.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
17.
Shaped rolling or section rolling
A variety of sections can be produced by roll forming process using a
series of forming rollers in a continuous method to roll the metal sheet to
a specific shape
Applications:
- construction materials,
- partition beam
- ceiling panel
- roofing panels.
- steel pipe
- automotive parts
- household appliances
- metal furniture,
- door and window frames
- other metal products.
www.formtak.com
A variety of rolled sections
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
18.
Ring rolling
Seamless rings
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
19.
Simulation of ring rolling
• The donut shape preform is placed
between a free turning inside roll and a
driven outside roll.
• The ring mills make the section thinner
while increasing the ring diameter.
www.qcforge.com
www.rz.rwth-aachen.de
Simulation
of ring
rolling
www.shape.co.kr Relative strain in ring rolling
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
20.
Seamless ring rolling
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
21.
Powder rolling
Metal powder is introduced between the rolls and compacted into a
‘green strip’, which is subsequently sintered and subjected to further
hot-working and/or cold working and annealing cycles.
Advantage :
- Cut down the initial hot-ingot breakdown step (reduced capital investment).
- Economical - metal powder is cheaply produced during the extraction process.
- Minimise contamination in hot-rolling.
- Provide fine grain size with a minimum of preferred orientation.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
22.
Continuous casting and hot rolling
• Metal is melted, cast and hot rolled continuously through a series of
rolling mills within the same process.
• Usually for steel sheet production.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
23.
Thread rolling
• Dies are pressed against the surface of cylindrical
blank. As the blank rolls against the in-feeding die
faces, the material is displaced to form the roots of
the thread, and the displaced material flows radially
outward to form the thread's crest.
• A blank is fed between two grooved die plates to form
the threads.
• The thread is formed by the axial flow of material in
the work piece. The grain structure of the material is
not cut, but is distorted to follow the thread form.
• Rolled threads are produced in a single pass at
speeds far in excess of those used to cut threads.
Cut thread and rolled
thread
Suranaree University of Technology
• The resultant thread is very much stronger than
a cut thread. It has a greater resistance to
mechanical stress and an increase in fatigue
strength. Also the surface is burnished and work
hardened.
Tapany Udomphol
Jan-Mar 2007
24.
Hot-rolling
Plate rolling
• The first hot-working operation for
most steel products is done on the
primary roughing mill (blooming,
slabbing or cogging mills).
• These mills are normally two-high
reversing mills with 0.6-1.4 m diameter
rolls (designated by size).
www.msm.cam.ac.uk
• The objective is to breakdown the cast ingot into blooms or slabs for
subsequent finishing into bars, plate or sheet.
• In hot-rolling steel, the slabs are heated initially at 1100 -1300 oC. The
temperature in the last finishing stand varies from 700 - 900 oC, but should
be above the upper critical temperature to produce uniform equiaxed
ferrite grains.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
25.
Example for hot strip mill process
www.nzsteel.co.nz
Red hot slab 210 mm
thick is ready for
rolling
Slabs are organised
according to rolling
schedule
Slab is reduced to a long strip
approx 25 mm thick
Oxidation scale is
removed
Mill reverses after each pass (5 or 7)
and the roll gap is reduced each time
The strip is coiled and uncoiled
to make the tail end lead
The strip is progressively reduced
to the required thicknesses
Leading edge and tail
end are removed
Plate 12 to 30 mm thick
Coiled steel 1.8 to 12 mm thk
910 mm to 1550 mm wide
Suranaree University of Technology
Strip is coiled and up ended or
passed through if heavy plate
Tapany Udomphol
Jan-Mar 2007
26.
• Flat plate of large thickness (10-50 mm) is
passed through different set of working
rolls, while each set consecutively reduces
thickness.
www.uksteel.org.uk
www.reverecopper.com
Plate rolling
• Hot strip is coiled to reduce its
increasing length due to a reduction of
thickness.
• Reducing the complication of controlling
strips of different speeds due to
different thicknesses. (thinner section
moves faster)
Hot rolled coil produced
on strip mill
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
27.
Cold-rolling
• Cold rolling is carried out under
recrystallisation temperature and
introduces work hardening.
• The starting material for cold-rolled steel
sheet is pickled hot-rolled breakdown coil
from the continuous hot-strip mill.
www.williamsonir.com
• The total reduction achieved by cold-rolling generally will vary from about
50 to 90%.
• The reduction in each stand should be distributed uniformly without falling
much below the maximum reduction for each pass.
• Generally the lowest percentage reduction is taken place in the last pass
to permit better control of flatness, gage, and surface finish.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
28.
Example for cold strip mill process.
www.nzsteel.co.nz
In batches of 9 coils, cold
rolled steel is annealed to
reduce work hardening
Coils are transferred to
and from the annealing
furnace
The 6 roll configuration enables this
high speed mill to produce steel of
high quality with consistent shape
and flatness
Cold rolling mill
The combination mill has a dual
function, cold rolling and single pass
temper rolling
Cold rolling reduces the thickness
and increases the strength of hot
rolled steel. The surface finish and
shape improve and work hardening
results
Temper rolling improves the shape
of the strip after its workability has
been improved by annealing
Cold rolled, annealed and
tempered coils are transferred
to the Cold Finishing Section
20 tonne coils of cold rolled
steel are dispatched to
Metal Coating Line
Coils up to 40 tones enter on a
conveyor from the pickle line
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
29.
Cold-rolling
• Cold rolling provide products with
superior surface finish (due to low
temperature
no oxide scales)
• Better dimensional tolerances
compared with hot-rolled products due
to less thermal expansion.
• Cold-rolled nonferrous sheet may be produced from
hot-rolled strip, or in the case of certain copper alloys
it is cold-rolled directly from the cast state.
Cold rolled metals are rated as ‘temper’
Cold rolled strips
• Skin rolled : Metal undergoes the least rolling ~ 0.5-1%
harden, still more workable.
• Quarter hard : Higher amount of deformation. Can be bent
normal to rolling direction without fracturing
• Half hard : Can be bent up to 90o.
• Full hard : Metal is compressed by 50% with no cracking.
Can be bent up to 45o.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
30.
Fundamental concept of metal rolling
1) The arc of contact between the rolls and the
metal is a part of a circle.
Assumptions
2) The coefficient of friction, µ, is constant in
theory, but in reality µ varies along the arc of
contact.
o
3) The metal is considered to deform
plastically during rolling.
R
α
ho
vo
x
y
x
y
vf
hf
Lp
o
4) The volume of metal is constant before and
after rolling. In practical the volume might
decrease a little bit due to close-up of pores.
5) The velocity of the rolls is assumed to be
constant.
6) The metal only extends in the rolling direction
and no extension in the width of the
material.
7) The cross sectional area normal to the
rolling direction is not distorted.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
31.
Forces and geometrical relationships
in rolling
o
• A metal sheet with a thickness ho enters
the rolls at the entrance plane xx with a
velocity vo.
R
α
ho
vo
y
x
x
vf
y
hf
Lp
• Given that there is no increase in
width, the vertical compression of the
metal is translated into an elongation in
the rolling direction.
o
bho vo = bhv = bh f v f
• It passes through the roll gap and leaves
the exit plane yy with a reduced thickness
hf and at a velocity vf.
…Eq.1
• Since there is no change in metal
volume at a given point per unit time
throughout the process, therefore
Where b is the width of the sheet
v is the velocity at any thickness h intermediate between ho and hf.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
32.
From Eq.1
bho vo = bh f v f
R
x
ho
y
vo
vf
x’
hf
Given that bo = bf
Lo
o t
y’
h
vo < vf
=h
Lf
f t
Then we have
vo ho = v f h f
When ho > hf , we then have vo < vf
The velocity of the sheet must steadily increase
from entrance to exit such that a vertical element
in the sheet remain undistorted.
Suranaree University of Technology
Tapany Udomphol
vo h f
=
ho
vf
…Eq.2
Jan-Mar 2007
33.
• At only one point along the surface of contact between the roll and the
sheet, two forces act on the metal: 1) a radial force Pr and 2) a tangential
frictional force F.
• If the surface velocity of the roll vr equal to the velocity of the sheet, this
point is called neutral point or no-slip point. For example, point N.
• Between the entrance plane (xx)
and the neutral point the sheet is
moving slower than the roll surface,
and the tangential frictional force,
F, act in the direction (see Fig) to
draw the metal into the roll.
• On the exit side (yy) of the neutral
point, the sheet moves faster than
the roll surface. The direction of the
frictional fore is then reversed and
oppose the delivery of the sheet
from the rolls.
Suranaree University of Technology
N point : vroll = vsheet
α
θ
β
Friction acts in
opposite directions
x
Pr
x
Tapany Udomphol
F N
y
y
Jan-Mar 2007
34.
Pr is the radial force, with a vertical
component P (rolling load - the load with
which the rolls press against the metal).
The specific roll pressure, p, is the rolling
load divided by the contact area.
p=
P
bL p
…Eq.3
Where b is the width of the sheet.
Lp is the projected length of the arc of contact.
(ho − h f )2
L p = R(ho − h f ) −
4
12
[
]
≈ R (ho − h f )
12
…Eq.4
L p ≈ R∆h
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
35.
• The distribution of roll pressure
along the arc of contact shows that the
pressure rises to a maximum at the
neutral point and then falls off.
R
ho
p
• The pressure distribution does not
come to a sharp peak at the neutral
point, which indicates that the neutral
point is not really a line on the roll
surface but an area.
A
• The area under the curve is
proportional to the rolling load.
N
vo
hf
B Friction hill in rolling
• The area in shade represents the
force required to overcome
frictional forces between the roll
and the sheet.
• The area under the dashed line
AB represents the force required to
deform the metal in plane
homogeneous compression.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
36.
Roll bite condition
The angle of
bite or the angle
α
of contact
Prsineα
α
Pr
Fcosα
α
F
For the workpiece to enter the throat
of the roll, the component of the
friction force must be equal to or
greater than the horizontal
component of the normal force.
F cos α ≥ Pr sin α
F sin α
≥
≥ tan α
Pr cos α
is a tangential friction force
is radial force
Suranaree University of Technology
F = µPr
Therefore
F
Pr
But we know
µ = tan α
…Eq.5
• If tan α > µ, the workpiece cannot be drawn.
• If µ = 0, rolling cannot occur.
Tapany Udomphol
Jan-Mar 2007
37.
Therefore Free engagement will occur when µ > tan α
Increase the effective values of µ
, for example grooving the rolls
parallel to the roll axis.
+
Using big rolls to reduce tan α or
if the roll diameter is fixed, reduce
the ho
α1>α2
α2
α1
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
38.
The maximum reduction
The critical variables are
Lp and h
R
B
ho
vo
Lp
A
α
R-a
C
From triangle ABC, we have
R 2 = L2p + ( R − a ) 2
L2p = R 2 − ( R 2 − 2 Ra + a 2 )
L2p = 2 Ra − a 2
a
D
h
As a is much smaller than R, we
can then ignore a2.
L p ≈ 2 Ra ≈ R∆h …Eq.6
A large diameter roll will permit a
thicker slab to enter the rolls than will
a small-diameter roll.
R∆h
µ = tan α =
≈
≈
R − ∆h / 2 R − ∆h / 2
Lp
Suranaree University of Technology
Where ∆h = ho – hf = 2a
∆h
R
Tapany Udomphol
(∆h )max = µ 2 R
…Eq.7
Jan-Mar 2007
39.
Problem with roll flattening
When high forces generated in rolling are transmitted to the workpiece through
the rolls, there are two major types of elastic distortions:
1) The rolls tends to bend along their length because the workpiece tends to
separate them while they are restrained at their ends.
thickness
variation.
2) The rolls flatten in the region where they contact the workpiece. The radius
R’. (roll flattening)
of the curvature is increased R
According to analysis by Hitchcock,
Rollling
CP '
R ' = R 1 +
b(ho − h f )
R
R‘
Roll flattening
Where C = 16(1-ν2)/πE = 2.16 x 10-11 Pa-1 for steel rolls.
P’ = rolling load based on the deformed roll radius.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
40.
Example: Determine the maximum possible reduction for coldrolling a 300 mm-thick slab when µ = 0.08 and the roll diameter is 600
mm. What is the maximum reduction on the same mill for hot rolling
when µ = 0.5?
(∆h )max = µ 2 R
From Eq.7,
For cold-rolling
(∆h )max = (0.08)2 (300) = 1.92mm
For hot-rolling
(∆h )max = (0.5)2 (300) = 75mm
Alternatively, we can use the relationship below
sin α =
Lp
=
R
∆h = 1.92mm
Suranaree University of Technology
R∆h
, α = tan −1 (µ )
R
Tapany Udomphol
Jan-Mar 2007
41.
Simplified analysis of rolling load
The main variables in rolling are:
• The roll diameter.
• The deformation resistance of the metal as influenced by metallurgy,
temperature and strain rate.
• The friction between the rolls and the workpiece.
• The presence of the front tension and/or back tension in the plane of the
sheet.
We consider in three conditions:
1) No friction condition
2) Normal friction condition
3) Sticky friction condition
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
42.
1) No friction situation
In the case of no friction situation, the rolling load (P)
is given by the roll pressure (p) times the area of contact
between the metal and the rolls (bLp).
'
P = pbL p = σ o b R∆h
…Eq.8
Where the roll pressure (p) is the yield stress in plane strain
when there is no change in the width (b) of the sheet.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
43.
2) Normal friction situation
In the normal case of friction situation in plane strain, the average
pressure p can be calculated as.
_
p
_ '
σo
Where Q
h
)
…Eq.9
= µLp/h
= the mean thickness between entry and exit from the rolls.
_
From Eq.8,
We have
(
1 Q
=
e −1
Q
P = p bL p
P=
2
3
_
1 Q
e − 1 b R∆h
Q
σo
Roll diameter
Suranaree University of Technology
(
)
…Eq.10
Rolling load
Tapany Udomphol
Jan-Mar 2007
44.
•Therefore the rolling load P increases with the roll radius R1/2,
depending on the contribution from the friction hill.
• The rolling load also increases as the sheet entering the rolls
becomes thinner (due to the term eQ).
• At one point, no further reduction in thickness can be achieved if
the deformation resistance of the sheet is greater than the roll
pressure. The rolls in contact with the sheet are both severely
elastically deformed.
• Small-diameter rolls which are properly stiffened against deflection
by backup rolls can produce a greater reduction before roll flattening
become significant and no further reduction of the sheet is possible.
Backup rolls
Example: the rolling of aluminium cooking foil.
Roll diameter < 10 mm with as many as 18
backing rolls.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
45.
• Frictional force is needed to
pull the metal into the rolls and
responsible for a large portion
of the rolling load.
• High friction results in high rolling load, a steep friction hill and great
tendency for edge cracking.
• The friction varies from point to point along the contact arc of the roll.
However it is very difficult to measure this variation in µ, all theory of
rolling are forced to assume a constant coefficient of friction.
• For cold-rolling with lubricants, µ ~ 0.05 – 0.10.
• For hot-rolling , µ ~ 0.2 up to sticky condition.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
46.
Example: Calculate the rolling load if steel sheet is hot rolled 30% from
a 40 mm-thick slab using a 900 mm-diameter roll. The slab is 760 mm wide.
Assume µ = 0.30. The plane-strain flow stress is 140 MPa at entrance and
200 MPa at the exit from the roll gap due to the increasing velocity.
ho − h f
ho
_
x100 = 30%
(40) − (h f )
(40)
h f = 28mm
h=
x100 = 30
Q=
2
µL p
_
=
=
'
o
σ =
(40) + (28)
= 34mm
2
µ R∆h
_
h
∆h = ho − h f = (40) − (28) = 12mm
From Eq.10
ho + h f
h
σ ' entrance + σ 'exit
2
=
(0.30) 450 x12
= 0.65
(34)
=
140 + 200
= 170 MPa
2
1 Q
P = σ (e − 1)b R∆h
Q
1
P = 170
e 0.65 − 1 (0.76) 0.45 x0.012 = 13.4 MN
(0.65)
'
o
(
Suranaree University of Technology
)
Tapany Udomphol
Jan-Mar 2007
47.
3) Sticky friction situation
What would be the rolling load if sticky friction occurs?
Continuing the analogy with compression in plane strain
L
a
' p
p =σ
+ 1 = σ 0 _ + 1
2h
4h
_
'
o
From Eq.8,
_
P = p bL p
From example;
R∆h
P =σ
+ 1b R∆h
_
4h
0.45 x0.012
P = 170
+ 1(0.76) 0.45 x0.012
4 x0.034
P = 14.6MN
'
o
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
48.
Example: The previous example neglected the influence of roll flattening
under very high rolling loads. If the deformed radius R’ of a roll under load is given
in Eq.11, using C = 2.16x10-11 Pa-1, P’ =13.4 MPa from previous example.
CP '
'
R = R 1 +
b(ho − h f
)
Where C = 16(1-ν2)/πE ,P’ = Rolling load
…Eq.11
(
based on the deformed roll radius.
)
2.16 x10 −11 13.4 x10 6
'
R = 0.451 +
= 0.464m
0.76 x0.012
Q=
µ R∆h
_
=
We now use R’ to calculate a
new value of P’ and in turn
another value of R’
0.30 464 x12
= 0.66
34
The difference between
h
the two estimations of R’
1
P '' = 170
e 0.66 − 1 0.76 0.464 x0.012 = 13.7 MN is not large, so we stop
0.66
the calculation at this
point.
2.16 x10 −11 (13.7 x10 6 )
''
R = 0.451 +
= 0.465m
0.76 x0.012
(
)
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
49.
Relationship of µ, rolling load and torque
N point : vroll = vsheet
α
θ
β
Friction acts in
opposite
directions
x
Pr
x
FN
y
Lp
y
• We have known that the location of the neutral
point N is where the direction of the friction force
changes.
• If back tension is applied gradually to the sheet,
the neutral point N shifts toward the exit plane.
• The total rolling load P and torque MT (per unit
of width b) is given by
Where µ is obtained by
measuring the torque and the
rolling load at constant roll speed
and reduction with the proper
back tension.
P
=
b
∫ pdx
0
MT
=
b
Lp
Lp
o
o
(µpdx )R = µR ∫ pdx = µR P
∫
b
thus
µ=
Suranaree University of Technology
Lp
MT
PR
Tapany Udomphol
Jan-Mar 2007
50.
Back and front tensions in sheet
• The presence of back and front
tensions in the plane of the sheet
reduces the rolling load.
• Back tension may be produced
by controlling the speed of the
uncoiler relative to the roll speed.
• Front tension may be created
by controlling the coiler.
• Back tension is ~ twice as
effective in reducing the rolling
load P as front tension.
• The effect of sheet tension on
reducing rolling pressure p can be
shown simply by
p = σ −σ h =
'
o
2
3
Back tension, σb
Uncoiler
Front tension, σf
Coiler
p
σ’o
σ’o- σb
σ ’o
σ’o- σf
• If a high enough back tension is applied,
the neutral point moves toward the roll exit
–> rolls are moving faster than the metal.
_
σ o − σ h …Eq.11
• If the front tension is used, the neutral
point will move toward the roll entrance.
Where σh = horizontal sheet tension.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
51.
Problems and defects in rolled
products
Defects from cast ingot before rolling
Defects other than cracks can result from defects introduced during the
ingot stage of production.
• Porosity, cavity, blow hole occurred in the cast ingot will be closed up
during the rolling process.
• Longitudinal stringers of non-metallic inclusions or pearlite banding
are related to melting and solidification practices. In severe cases, these
defects can lead to laminations which drastically reduce the strength in the
thickness direction.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
52.
Defects during rolling
There are two aspects to the problem of the shape of a sheet.
1) Uniform thickness over the width and thickness – can be precisely
controlled with modern gage control system.
h
h
2) Flatness – difficult to measure accurately.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
53.
Uniform thickness
• Under high rolling forces, the rolls flatten
and bend, and the entire mill is elastically
distorted.
• Mill spring causes the thickness of the
sheet exiting from the rolling mill to be
greater than the roll gap set under no-load
conditions.
• Precise thickness rolling requires the
elastic constant of the mill. Calibration
curves are needed, see Fig.
(1–3 GNm-1 for screw-loaded rolling mills, 4
GNm-1 for hydraulically loaded mills).
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
54.
• Roll flattening increases the roll pressure and eventually causes
the rolls to deform more easily than the metal.
•The limiting thickness is nearly proportional to µ, R, σ’o but
inversely proportional to E.
For example in steel rolls the limiting thickness is given by
_ '
hmin =
µR σ o
…Eq.12
12.8
In general, problems with limiting gauge can be expected when the
sheet thickness is below 1/400 to 1/600 of the roll diameter.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
55.
Flatness
• The roll gap must be perfectly parallel to produce sheets/plates
with equal thickness at both ends.
• The rolling speed is very sensitive to flatness. A difference in
elongation of one part in 10,000 between different locations in the
sheet can cause waviness.
g n
lin tio
ol
R irec
d
Perfectly flat
More elongated
along edges
Suranaree University of Technology
More elongated in
the centre
Tapany Udomphol
Jan-Mar 2007
56.
Solutions to flatness problems
• Camber and crown can be used to correct the roll deflection (at only one
value of the roll force). Or use rolling mill equipped with hydraulic jacks to
permit the elastic distortion of the rolls to correct deflection.
(a)
(b)
(a) The use of cambered rolls to compensate for roll bending.
(b) Uncambered rolls give variation of thickness.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
57.
•The roll cross angle of rolls incorporated
in a stand of each rolling mill is set at a
predetermined value beforehand.
• If there is a roll cross angle that will
enable a target sheet crown to be applied
to each sheet and the roll bender load of
each stand is adjusted on-line, thereby
effecting sheet crown control.
• Hot mill can be provided with
facilities for crown control to
improve the control of the
profile of hot strip mill.
• For example work roll
bending with continuous
variable crown and pair cross
mills.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
58.
Possible effects when rolling with insufficient camber
(a)
(b)
(c)
(d)
(e)
• Thicker centre means the edges would be plastically elongated more
than the centre, normally called long edges.
• This induces the residual stress pattern of compression at the edges
and tension along the centreline.
• This can cause centreline cracking (c), warping (d) or edge
wrinkling or crepe-paper effect or wavy edge (e).
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
59.
Possible effects when rolls are over-cambered.
(b)
(a)
(c)
(d)
(e)
• Thicker edges than the centre means the centre would be plastically
elongated more than the edges, resulting in lateral spread.
•The residual stress pattern is now under compression in the centreline and
tension at the edges (b).
• This may cause edge cracking (c), centre splitting (d), centreline
wrinkling (e).
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
60.
• Shape problems are greatest when rolling in thin strip (<0.01 in)
because fractional errors in the roll gap profile increase with
decrease in thickness, producing larger internal stress.
• Thin sheet is also less resistant to buckling.
• Mild shape problems may be corrected by stretch levelling the
sheet in tension or by bend flexing the sheet in a roller-leveller,
see Fig.
two high
adjustable
Material
flow
work rolls
Roller-leveller
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
61.
• Edging can also be caused by inhomogeneous deformation in the
thickness direction.
• If only the surface of the workpiece is deformed (as in a light reduction on a
thick slab), the edges are concaved (a). The overhanging material is not
compressed in the subsequent step of rolling, causing this area under tensile
stress and leading to edge cracking. This has been observed in initial
breakdown of hot-rolling when h/Lp > 2
• With heavy reduction, the centre tends
to expand more laterally than the surface
to produced barrelled edges (b). This
causes secondary tensile stresses by
barrelling, which are susceptible to edge
cracking.
• Alligatoring (c) will occur when lateral
spread is greater in the centre than the
surface (surface in tension, centre in
compression) and with the presence of
metallurgical weakness along the
centreline.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
62.
• Surface defects are more easily in rolling due to high surface to
volume ratio. Grinding , chipping or descaling of defects on the
surface of cast ingots or billets are recommended before being
rolled.
• Laps due to misplace of rolls can cause undesired shapes.
Roll
misplacement
• Flakes or cooling cracks along edges result in decreased ductility in hot
rolling such as blooming of extra coarse grained ingot.
• Scratches due to tooling and handling.
• Variation in thickness due to deflection of rolls or rolling speed.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
63.
Rolling mill control
• Modern continuous hot-strip and cold rolling mills operated under
automatic control provide high throughput and production rate.
• Of all the metal working processes, rolling is the best suited for the
adoption of automatic control because it is an essentially steady-state
process in which the tooling geometry (roll gap) may be changed readily
during the process.
• Automatic control in rolling such as the development of online sensors
to continuously measure sheet thickness. The most widely used
instruments are
1) flying micrometer
2) x-ray or isotope, gauges which measure thickness by monitoring
the amount of radiation transmitted through the sheet.
• More recently control procedures have been aimed at controlling strip
shape as well as thickness.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
64.
Problem of gauge control
Normal situation
Plastic curve
Rolling load
Elastic curve
• For a given set of rolling conditions, the
rolling load varies with the final sheet
thickness, according to the plastic
curve, which can be obtained in Eq.10.
P
1 Q
P=
σ o e − 1 b R∆h
3 Q
2
Roll gap
hf
ho
Sheet thickness
Characteristic elastic and plastic
curves for a rolling mill
Suranaree University of Technology
_
(
)
• The elastic curve for mill spring
indicates that a sheet of initial thickness
ho will have a final thickness hf and the
load on the mill would be P in normal
situation.
Tapany Udomphol
Jan-Mar 2007
65.
Situation where µ or flow stress increase
Rolling load
Increase in
µ or σ
µ
due to lubricant breakdown
σ
due to Temp
Elastic
curve
P3
P2
P1
The plastic curve will be raised.
Therefore rolling load
P1
final thickness hf1
New
roll gap
hf1hf2 ho
Sheet thickness
Use of characteristic curves to show
changes in rolling condition.
P2
hf2
In order to maintain a constant thickness hf1,
under these new condition, the roll gap
would have to be decreased. This moves the
elastic curve to the left and further
increases the rolling load to P3.
Example: • If the sheet thickness increases, the plastic curve will move to the
right relative to the elastic curve.
• If the there is an increase in strip tension, the plastic curve will move
to the left.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
66.
Thickness measurement in continuous hot mill
• In a continuous hot mill, the strip thickness is measured indirectly
by measuring the rolling load and using the characteristic curve of
the mill to establish the thickness.
• The error signal is fedback to the rolling mill screws to reposition them
so as to minimise the error.
• An x-ray gauge is used after the last stand to provide an absolute
measurement of sheet gauge.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
67.
Thickness measurement in continuous
cold strip mills
• Thickness is measured by x-ray
gauges while the error in the
thickness following the first stand is
usually fedback to adjust the gap
sitting on the first stand.
• Gauge control in subsequent stands
usually is achieved by controlling the
strip tension through controlling the
relative roll speed in successive stands
or the coiler speed.
• Gauge control through control of
strip tension has faster response
time than control through change in
roll setting.
Suranaree University of Technology
sensors
Thickness gauging is achieved
by using two opposing
sensors with laser spots
aimed at opposite sides of a
target. The sensor readings
are subtracted from the sensor
separation distance to yield a
real-time thickness
measurement.
Tapany Udomphol
Jan-Mar 2007
68.
Theory of cold rolling
A theory of rolling is aimed at expressing the external forces, such as
the rolling load and the rolling torque, in terms of the geometry of the
deformation and the strength properties of the material being rolled.
Assumptions
1) The arc of the contact is circular – no elastic deformation of the roll.
2) The coefficient of friction is constant at all points on the arc of contact.
3) There is no lateral spread, so that rolling can be considered a problem
in plain strain.
4) Plane vertical section remain plane: i.e., the deformation is
homogeneous.
5) The peripheral velocity of the rolls is constant
6) The elastic deformation of the sheet is negligible in comparison with the
plastic deformation.
7) The distortion-energy criterion of yielding, for plane strain, holds.
σ1 − σ 3 =
Suranaree University of Technology
2
3
'
σo =σo
Tapany Udomphol
Yield stress in plane
strain condition
Jan-Mar 2007
69.
The stresses acting on an element of strip in the roll gap
o
ho
µPr
h+dh h
hf
µPrsinθ
σx
Prcosθ
dθ
σx+dσx
θ
µPrcosθ
θ
Pr
Prsinθ
R dθ
B
• At any point of contact between the strip and the roll surface, designated
by the angle θ, the stresses are the radial pressure pr and the
tangential shearing stress τ = µpr. These stresses are resolved into
their horizontal and vertical components (b).
• The stress σx is assumed to be uniformly distributed over the vertical
faces of the element.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
70.
Rd
Rd
θ
Pr
µPrcosθ
Prcosθ
θ Pr
µPrsinθ
σx
µPr
Pr
µPrcosθ
µPrcosθRdθ
h
PrsinθRdθ
θ θ
σxh
(σx+dσx)(h+dh)
µPrcosθRdθ
U
ni
tl
en
gt
h
θ
θ
θ
θ
h+dh σx+dσx
Prsinθ
µ
µ
θ
θ
θ
µPrsinθ
µ
Prcosθ
θ
PrsinθRdθ
θ θ
Prsinθ
R dθ
Taking summation of the horizontal forces on the element results in
(σ x + dσ x )(h + dh ) + 2µp r cos θRdθ = σ x h + 2 p r sin θRdθ
Which simplifies to
d (σ x h )
= 2 p r R(sin θ ± µ cos θ )
dθ
Suranaree University of Technology
Tapany Udomphol
…Eq.14
Jan-Mar 2007
71.
The forces acting in the vertical direction are balanced by the specific roll
pressure p. Taking the equilibrium of forces in the vertical direction results in
a relationship between the normal pressure and the radial pressure.
p = p r (1 m µ tan θ )
…Eq.14
The relationship between the normal pressure and the horizontal
compressive stress σx is given by the distortion energy criterion of
yielding for plane strain.
σ1 − σ 3 =
2
3
'
σo =σo
'
p −σ x = σo
…Eq.15
Where p is the greater of the two compressive principal stresses.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
72.
The solution of problems in cold rolling are complicated. Some
simplification to this problem has been provided by Bland and Ford.
By restricting the analysis to cold rolling under conditions of low
friction and for angles of contact < 6o, then we can put sin θ ~ θ
and cos θ ~ 1. Thus Eq.14 can be written
d (σ d h )h) = 2 p R (θ '± µ )
x (σ
dθ = 2 p r R (θ ± µ )
dθ
'
x
…Eq.16
r
It is also assumed that pr ~ p , so that Eq.15 can be written σx = pr-σ’o.
By substituting into Eq.16 and integrating, relatively simple equations of
the radial pressure result.
Roll entrance to neutral point:
'
σ oh
Neutral point to roll exit:
σ
1 − xb e µ ( H − H ) …Eq.17
pr =
'
ho σ 01
Where
R'
H = 2
h
f
1
1
2
'
−1 R
tan
h f
Suranaree University of Technology
1
2
θ
σ xf µH
1 − ' e
pr =
h f σ 02
'
σ oh
…Eq.18
and σxb = back tension
σxf = front tension
Tapany Udomphol
Jan-Mar 2007
73.
The rolling load or total force P is the integral of the specific roll
pressure over the arc of contact.
θ =α
P = R 'b
∫ pdθ
…Eq.19
o
Where
b = width of sheet
α = contact angle
The solution is replaced by the modern digital computer.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
74.
Theory of hot-rolling
In hot working processes, the flow stress for hot-rolling is a function of
both temperature and strain rate (speed of rolls)
Calculation of rolling load by Sims
[
P = σ b R (ho − h f
'
o
)]
1
2
Qp
…Eq.20
Where Qp is a complex function of
the reduction in thickness and the
ratio R/hf. Values of Qp may be
obtained from
Qp =
2
ho
hn
R
∆h
−1
−
ln
π tan
4∆h
hf
hf
ho h f
π
−
4
…Eq.21
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
75.
Torque and power
Torque is the measure of the force applied to a member to produce
rotational motion.
Power is applied to a rolling mill by applying a torque to the rolls and by
means of strip tension.
The power is spent principally in four ways
1)
2)
3)
4)
The energy needed to deform the metal.
The energy needed to overcome the frictional force.
The power lost in the pinions and power-transmission system.
Electrical losses in the various motors and generators.
Remarks: Losses in the windup reel and uncoiler must also be considered.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
76.
The total rolling load is distributed
over the arc of contact in the typical
friction-hill pressure distribution.
However the total rolling load can be
assumed to be concentrated at a
point along the act of contact at a
distance a from the line of centres of
the rolls.
a
R
P
a
=
Lp
a
R∆h
…Eq.22
hf
ho
P
The ratio of the moment arm a to the
projected length of the act of contact
Lp can be given as
λ=
MT = Pa
a
R
Schematic diagram illustrating roll torque
Where λ is 0.5 for hot-rolling and 0.45 for cold-rolling.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
77.
The torque MT is equal to the total rolling
load P multiplied by the effective moment
arm a. Since there are two work rolls, the
torque is given by
M T = 2 Pa
…Eq.23
MT = Pa
a
R
P
During one revolution of the top roll the
resultant rolling load P moves along the
circumference of a circle equal to 2πa.
Since there are two work rolls, the work
done W is equal to
Work = 2(2πa) P
hf
ho
P
a
R
…Eq.24
Since power is defined as the rate of doing work, i.e., 1 W = 1 J s-1, the
power (in watts) needed to operated a pair of rolls revolving at N Hz (s-1) in
deforming metal as it flows through the roll gap is given by
W = 4πaPN
…Eq.25
Where P is in newtons and a is in metres.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
78.
Example: A 300 mm-wide aluminium alloy strip is hot-rolled in thickness from
20 to 15 mm. The rolls are 1 m in diameter and operate at 100 rpm. The uniaxial
flow stress for aluminium alloy can be expressed as σ = 140ε0.2 (MPa).
Determine the rolling load and the power required for this hot reduction.
From Eq.20
[
'
P = σ o b R (ho − h f
1
2
b = 0.3 m, R = 0.5 m, ho = 0.02 m and hf
= 0.015 m, we need to know σ’o and Qp.
Qp
ε1
20
ε 1 = ln = 0.288
15
20 − 15
r=
= 0.25
20
R 500
=
= 33.3
hf
15
P=
)]
'
σo =
k ∫ ε n dε
o
ε1
kε n +1
=
ε 1 (n + 1)
140(0.288)
σ =
1.2
ε1
o
kε 1n
=
n +1
0.2
'
o
2
3
= 91MPa
(91)(0.3)[0.5(0.020 − 0.015)]
1
2
Qp can be found
from graph(~1.5)
when reduction r and
R/hf are known.
(1.5) = 2.36MN
a = 0.5 R∆h = 0.5 0.5 x0.005 = 0.025m
N = 100 / 60 = 1.67 s −1
(
)
W = 4π (0.025) 2.36 x10 −6 (1.67 )Js −1 = 1.24MW
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
79.
References
• Dieter, G.E., Mechanical metallurgy, 1988, SI metric edition,
McGraw-Hill, ISBN 0-07-100406-8.
• Edwards, L. and Endean, M., Manufacturing with materials, 1990,
Butterworth Heinemann, ISBN 0-7506-2754-9.
• Beddoes, J. and Bibbly M.J., Principles of metal manufacturing
process, 1999, Arnold, ISBN 0-470-35241-8.
• Lecture note, 2003.
• Firth Rixson leavelets.
• Metal forming processes, Prof Manas.
• Metal forming lecture, Ass Prof. P. Srichareonchai.
Suranaree University of Technology
Tapany Udomphol
Jan-Mar 2007
Views
Actions
Embeds 0
Report content